2 International Journal of Corrosion
Table 1: Eﬀect of concentration of trans-4-hydroxy-4 -stilbazole on the corrosion rate (mg·cm−2·h−1) and percentage eﬃciency of mild
steel in 1 M HCl at various temperatures.
303 313 323 333 343
1 M HCl 0.961 — 1.394 — 4.671 — 12.225 — 26.280 —
1 M HCl + 1 × 10−7 M 0.950 1 1.381 0.9 4.648 0.5 14.057 −15 28.139 −7.1
1 M HCl + 1 × 10−6 M 0.916 5 1.343 3.7 4.570 2.2 12.733 −4 27.061 −3.0
1 M HCl + 1 × 10−5 M 0.714 26 1.203 14 4.192 10.3 12.714 −4 24.901 5.2
1 M HCl + 1 × 10−4 M 0.191 80 0.361 74 2.179 53.4 8.959 27 24.020 8.6
1 M HCl + 1 × 10−3 M 0.060 94 0.112 92 0.543 88.4 2.321 81 8.619 67
inhibition of mild steel in 1 M HCl solution. Mild steel was
chosen in our studies since high-temperature aggressive acids
are widely used in industries in connection to mild and low
In this work, trans-4-hydroxy-4 -stilbazole was prepared
via a synthesis which produced a high percentage yield of this
The aim of this work is to study, using weight loss
measurements, the eﬀect of temperature on the corrosion
inhibition of mild steel in 1 M HCl solution by trans-
4-hydroxy-4 -stilbazole, a synthesized compound that was
previously studied using electrochemical technique  and
found to be a very eﬃcient corrosion inhibitor, and to
calculate the thermodynamic parameters. Hence, the output
of this study is intended to be the building block or the
nucleus for a new family or group of stilbazole derivatives
in all studies of corrosion inhibitors.
2. Experimental Details
2.1. Instrumentation. The experimental setup consisted of a
250 mL round bottom ﬂask ﬁtted with a reﬂux condenser and
a long glass rod on which the specimen was hooked and in
turn immersed in a thermally controlled water bath [28, 42].
Analytical-grade hydrochloric acid (Ajax), 4-iodophenol,
triethylamine, palladium acetate, tri(o-tolyl)phosphine, ace-
tonitrile, dichloromethane, MgSO4, hexane, and pentane
were obtained from Aldrich Chemical Company and used
without further puriﬁcation. 4-Vinylpyridine was distilled
under reduced pressure and stored in cold place.
2.2. Sample Preparation. Rectangular specimens (1 cm ×
2.3 cm × 0.3 cm) cut from large sheet of 3 mm thick mild
steel (IS 226 containing 0.18% C, 0.6% Mn, and 0.35% Si)
supplied by “Reliable Steel Traders,” Sharjah, UAE, were used
for weight loss measurements. A 2 mm diameter hole was
drilled close to the upper edge of the specimen and served
to be hooked with a glass rod for immersion purposes. Prior
to each experiment, the specimens were polished with 600
grade emery paper, rinsed with distilled water, degreased
with acetone, dried, and ﬁnally weighed precisely on an
accurate analytical balance.
2.3. Synthesis of Trans-4-Hydroxy-4 -Stilbazole. Several
methods for the synthesis of trans-4-hydroxy-4 -stilbazole
are available including the reaction of 4-picoline with
4-Hydroxy benzaldehyde in acetic anhydride [43, 44], which,
under such conditions, gave only tiny yields after long
reactions. A better procedure was developed and which
used Heck-type vinylic addition reaction  catalyzed by
palladium. Using this procedure, we were able to obtain a
yield of about 80% and quantities reaching up to 20 g in one
single reaction, following the modiﬁed procedure set by 
and described in our previous work .
2.4. Measuring Procedure. The ﬂask was ﬁlled with 100 mL
of 1 M HCl solution either with or without trans-4-hydroxy-
4 -stilbazole of various concentrations, then placed in water
bath. As soon as the required working temperature was
reached, the mild steel sample was immersed in the solution,
and left there for exactly six hours, after which the sample was
removed, rinsed with distilled deionized water, degreased
with acetone, dried, and ﬁnally weighed precisely on an
accurate analytical balance. This procedure was repeated
with all the samples with a variety of inhibitor concentrations
ranging from 1×10−7 M up to 1×10−3 M, and at tempera-
tures ranging from 303 K to 343 K.
Weight loss corrosion tests were carried out on the mild steel
in 1 M HCl in the absence or presence of trans-4-hydroxy-
4 -stilbazole over a period of 6 hours. Table 1 represents
the corrosion rates [mg·cm−2·h−1] and the percentage
eﬃciencies for the studied inhibitor with concentrations
varying from 1×10−7 M to 1×10−3 M at 303, 313, 323,
333, and 343 K, respectively. The percentage eﬃciency was
calculated according to the following expression:
% Inhibition =
WUninh. − WInh.
× 100, (1)
where WUninh. is corrosion rate without inhibitor and WInh.
is corrosion rate with inhibitor.
Figures 1 and 2 show the plots of the corrosion rate of
trans-4-hydroxy-4 -stilbazole as a function of concentration
International Journal of Corrosion 3
1E−011E−07 1E−05 1E−03
Figure 1: Eﬀect of concentration of trans-4-hydroxy-4 -stilbazole
on the corrosion rate (mg·cm−2·h−1) of mild steel in 1 M HCl at
at 303, 313, 323, 333, and 343 K. At 303 K (Figure 1), the
corrosion rate dropped from 0.961 mg·cm−2·h−1 (1 M HCl
in the absence of the inhibitor) to 0.950 mg·cm−2·h−1 when
1×10−7 M of trans-4-hydroxy-4 -stilbazole was present in
the 1 M HCl. This corrosion rate continued to decrease
slightly to reach 0.714 mg·cm−2·h−1 (26% inhibition) at a
concentration of 1×10−5 M, followed by a steep decrease
to reach 0.191 mg·cm−2·h−1 when the inhibitor’s concen-
tration was 1×10−4 M, and ﬁnally, at higher concentration
(1×10−3 M) the corrosion rate as initially decreased slightly
to reach 0.060 mg·cm−2·h−1 (94% inhibition). At 313 K
(Figure 1), the curve showed to have similar shape as that
obtained at 303 K. At concentrations greater than 1×10−5 M,
the corrosion rate decreased steeply and reached about
0.112 mg·cm−2·h−1 (92%) at 1×10−3 M.
At 323 K (Figure 2), when the concentration of the inhib-
itor was between 1×10−7 M and 1×10−5 M, it had very slight
eﬀect on the corrosion rate; whereas at higher concentra-
tions, the corrosion rate dropped from 4.192 mg·cm−2·h−1
(at 1×10−5 M) down to 2.179 and 0.543 mg·cm−2·h−1 at
1×10−4 M and 1×10−3 M, respectively.
At 333 K (Table 1), the presence of trans-4-hydroxy-4 -
stilbazole acted as an accelerator between 1×10−7 M and
1×10−5 M, and at concentrations of 1×10−4 M and greater, it
acted as inhibitor reaching percentage inhibitions of 27% and
81% at 1×10−4 M and 1×10−3 M, respectively. At 343 K, like-
wise, trans-4-hydroxy-4 -stilbazole acted as an accelerator
between 1×10−7 M and 1×10−6 M, then inhibited the mild
steel at 1×10−5 M and greater concentration, reaching a per-
centage inhibition of about 67% at 1×10−3 M. It was noticed
that a tenfold increase in the inhibitor’s concentration,
1E−011E−07 1E−05 1E−03
Figure 2: Eﬀect of concentration of trans-4-hydroxy-4 -stilbazole
on the corrosion rate (mg·cm−2·h−1) of mild steel in 1 M HCl at
namely, from 1×10−4 M to 1×10−3 M, had a very sizeable
increase in the percentage inhibition as this increased from
27% to 81% at 333 K, and from 8.6% to 67% at 343 K.
Figure 3 shows the plots of the percent inhibition versus
the concentration of the inhibitor at temperatures of 303,
313, 323, 333, and 343 K, respectively. This ﬁgure showed
that the percent inhibition was not suﬃciently aﬀected by
the increase of temperature (303 to 323 K), especially when
low concentrations (1×10−7 to 1×10−5 M) of inhibitors
were employed; whereas at higher concentrations (above
1×10−5 M), the presence of the inhibitor greatly increased
the percent inhibition at all temperatures. At higher tem-
peratures, it was noticed that at concentrations between
1×10−7 M and 1×10−4 M (343 K) and in some cases to
1×10−5 M (333 K) trans-4-hydroxy-4 -stilbazole acted as a
The data obtained from the weight loss measurements
were plotted in accordance to Arrhenius equation:
ln rate = −
+ const., (2)
where Ea is activation energy [kcal·mol−1], R is gas constant
[kcal·mol−1], T is absolute temperature [K], and const. is
Figure 4 represents the Arrhenius plot of the corrosion of
mild steel in 1 M HCl solution (ln corrosion rate as a function
of 1/T) with or without the presence of trans-4-hydroxy-
4 -stilbazole at concentrations ranging from 1×10−7 M to
1×10−3 M. From this ﬁgure, the slope (−Ea/R) of each
4 International Journal of Corrosion
1E−07 1E−05 1E−03
Inhibitor concentration (M)
Figure 3: Eﬀect of concentration of trans-4-hydroxy-4 -stilbazole
on the percent inhibition of mild steel in 1 M HCl at various
individual line was determined and used to calculate the
activation energy according to (2), and taking R = 1.987 ×
10−3 kcal·mol−1 (Table 2). The increase of concentration of
trans-4-hydroxy-4 -stilbazole (from 1×10−7 M to 1×10−3 M)
increased the activation energies for the corrosion of mild
steel in 1 M HCl (initially 18.27 kcal·mol−1) (Table 2).
Table 3 shows the surface coverage of various concen-
trations of trans-4-hydroxy-4 -stilbazole (from 1×10−7 M to
1×10−3 M) on mild steel surface as a function of temper-
ature. These values were extracted from the corresponding
percent eﬃciency values reported earlier in Table 1. The
plot of surface coverage, θ, against the natural logarithm
of the concentration of the inhibitor, ln C, for mild steel
at various inhibitor temperatures is shown in Figure 5.
After examining these data and adjusting them to diﬀerent
theoretical adsorption isotherms, it was concluded that the
inhibitor was adsorbed on the mild steel surface according to
−2aθ = lnKC, (3)
where a is molecular interaction constant, θ is degree of
coverage, K is equilibrium constant for the adsorption
reaction, and C is concentration of the inhibitor. The
equilibrium constant for the adsorption reaction, K, is
related to the standard free energy of adsorption  via:
2.8 3 3.2 3.4
(1/T) × 103 (K−1)
Figure 4: Eﬀect of temperature on the corrosion rate of mild steel
in 1 M HCl solution with and without the presence of various
concentrations of trans-4-hydroxy-4 -stilbazole inhibitor.
where K is equilibrium constant for the adsorption reaction,
55.5 is concentration of water [mol·L−1], ΔG is standard free
energy [kcal·mol−1], R is gas constant [kcal·mol−1], and T is
absolute temperature [K].
According to (3), the straight lines shown in Figure 5 will
have the following slopes and intercepts:
Slope = −
Intercept = −
Combination of (5) and (6) leads to the following relation-
Intercept = Slope · (lnK), (7)
from which the equilibrium constant for the adsorption
reaction, K, can be calculated:
K = e(Intercept/Slope)
The free energy of adsorption of the inhibitor, ΔG, can be
calculated from the results in Figure 5 used to calculate the
equilibrium constant, K, and (4) at various temperatures
(303 K to 323 K).
The enthalpy of adsorption, ΔH, for the inhibitor can be
calculated from the following equation:
ΔH = Ea − RT. (9)
International Journal of Corrosion 5
Table 2: The activation energy (Ea) for the corrosion of mild steel in 1 M HCl with and without trans-4-hydroxy-4 -stilbazole inhibitor at
Activation energy, Ea (kcal·mol−1)
1 × 10−3 M 1 × 10−4 M 1 × 10−5 M 1 × 10−6 M 1 × 10−7 M
1 M HCl 18.27 18.27 18.27 18.27 18.27
1 M HCl+trans-4-hydroxy-
26.93 26.82 19.72 18.76 18.93
Table 3: Eﬀect of concentration of trans-4-hydroxy-4 -stilbazole on
surface coverage for mild steel in 1 M HCl at various temperatures.
303 313 323
1 M HCl + 1 × 10−6 M 0.05 0.037 0.022
1 M HCl + 1 × 10−5 M 0.26 0.14 0.103
1 M HCl + 1 × 10−4 M 0.80 0.74 0.534
1 M HCl + 1 × 10−3 M 0.94 0.92 0.884
The entropy, ΔS, can be calculated at various temperatures
for the inhibitor using the following equation:
ΔG = ΔH − TΔS. (10)
The results in Table 2 show that the activation energy (Ea)
for the corrosion of mild steel in the presence of the inhibitor
are higher compared to the activation energy in the absence
of inhibitor at both 1 × 10−3 M and 1 × 10−4 M (about 27
versus about 18 kcal·mol−1). Whereas at lower concentration
(from 1 × 10−5 to 1 × 10−7 M), the activation energy is
very close to that in uninhibited HCl solution. This can be
attributed to the fact that higher values of Ea in the presence
of inhibitor compared to its absence are generally consistent
with a physisorption, while unchanged or lower values of Ea
in inhibited solution suggest charge sharing or transfer from
the organic inhibitor to the metal surface to form coordinate
covalent bonds (chemisorption).
The increase in the activation energies for the corrosion is
attributed to a decrease in the adsorption of the inhibitor on
the metal surface as the temperature increased; subsequently,
an increase in the corrosion rate will result due to the greater
exposed area of the metal surface to the acid.
Tables 4, 5, and 6 show the thermodynamic data obtained
in the presence of the inhibitor at various temperatures.
These thermodynamic quantities represent the algebraic
sum of the values for adsorption and desorption. The
negative value of ΔG indicates the spontaneous adsorption
of inhibitor on the surface of the mild steel. The free
energy, ΔG, varies from −11.54 kcal·mol−1 at 303 K to
−11.12 kcal·mol−1 at 323 K. The adsorption process is
believed to be exothermic and associated with a decrease in
entropy (ΔS) of solute, while the opposite is true for the
solvent . The gain in entropy which accompanies the
−16 −12 −8
Ln concentration (M)
Figure 5: Eﬀect of concentration of trans-4-hydroxy-4 -stilbazole
on the surface coverage of mild steel in 1 M HCl at various
Table 4: The enthalpy of adsorption (ΔH) for mild steel in 1 M HCl
in the presence of 1×10−3 M trans-4-hydroxy-4 -stilbazole inhibitor
at various temperatures (303 K–343 K).
303 K 313 K 323 K 333 K 343 K
26.33 26.31 26.29 26.27 26.25
substitutional adsorption process is attributed to the increase
in the solvent entropy (Table 6). This agrees with the general
suggestion that the values of ΔG increase with the increase
of inhibition eﬃciency [20, 26] as the adsorption of organic
compound is accompanied by desorption of water molecules
oﬀ the surface.
The electron density group (–OH) on the phenyl ring
gives an extra inhibition eﬀect. The high inhibition eﬃciency
may be attributed to the preferred ﬂat orientation of this
compound on the metal surface. The interaction occurs
6 International Journal of Corrosion
Table 5: The free energy of adsorption (ΔGads) for mild steel in
1 M HCl in the presence of trans-4-hydroxy-4 -stilbazole inhibitor
at various temperatures (303 K–323 K).
303 K 313 K 323 K
−11.54 −11.76 −11.12
Table 6: The change in entropy (ΔS) for mild steel in 1 M HCl
in the presence of trans-4-hydroxy-4 -stilbazole inhibitor at various
temperatures (303 K–323 K).
303 K 313 K 323 K
0.125 0.122 0.116
between the delocalized π-electrons of the two rings, the
double bond (–C=C–), and the lone pair of electrons on
N and O atoms with the positively charged metal surface.
In addition, (–C=C–) bond plays the major role in the
stabilization of both sides of the Stilbazole structure.
These results agree with  who suggested that the
inhibition eﬃciency of organic compounds depends on
many factors including their charge density, number of
adsorption sites, heat of hydrogenation, mode of interaction
with the metal surface, and formation of metallic complexes
Trans-4-hydroxy-4 -stilbazole was found to be a highly eﬃ-
cient inhibitor for mild steel in 1.0 M HCl solution, reaching
about 94% at 1.0 × 10−3 M and 303 K, a concentration
considered to be very moderate.
Trans-4-hydroxy-4 -stilbazole is a potential corrosion
inhibitor since it contains not only nitrogen and oxygen, but
also phenyl and pyridine rings that are joined together with a
double bond (–C=C–) in conjugation with these rings. It was
apparent from the molecular structure that this compound
would be adsorbed onto the metal surface through the lone
pair of electron of nitrogen and oxygen and pi electrons of
the two aromatic rings (phenyl and pyridine) and the double
bond that join them together.
The percentage of inhibition in the presence of this
inhibitor was decreased with temperature, which indicates
that physical adsorption was the predominant inhibition
mechanism because the quantity of adsorbed inhibitor
decreases with increasing temperature.
 B. B. Damaskin, O. A. Pietrij, and W. W. Batrokov, “Adsorpcja
organiczeskich sojedinienij na electrodach,” Moskva, 1968.
 G. Okamoto, M. Nagayama, J. Kato, and T. Baba, “Eﬀect of
organic inhibitors on the polarization characteristics of mild
steel in acid solution,” Corrosion Science, vol. 2, no. 1, pp. 21–
 S. M. Beloglazov, Z. I. Dzhafarov, V. N. Polyakov, and N.
N. Demushia, “Quaternary ammonium salts as corrosion
inhibitors of steel in the presence of sulfate-reducing bacteria,”
Protection of Metals USSR, vol. 27, no. 6, pp. 810–813, 1991.
 A. V. Fokin, M. V. Pospelov, and A. N. Levichev, “Structural
and protective capacities of organic corrosion inhibitors. 2.
Alkylethylene diamines and quaternary ammonium salts,”
Protection of Metals USSR, vol. 19, no. 2, pp. 242–244, 1983.
 A. H. Nahl´e, “Electrochemical studies of corrosion inhibition
of a series of quaternary ammonium salts on iron in HCl
solution,” Corrosion Prevention and Control, vol. 44, no. 4, pp.
 A. H. Nahl´e, “Inhibition of iron in HCl using benzyl trimethyl-
and triethyl-ammonium chlorides,” Corrosion Prevention and
Control, vol. 45, no. 4, pp. 124–130, 1998.
 A. Nahl´e, “Eﬀect of triethanolamine on the electrochemical
dissolution of solder in NaOH solution,” Bulletin of Electro-
chemistry, vol. 18, no. 3, pp. 105–110, 2002.
 A. Nahle and F. C. Walsh, “Electrochemical studies of two cor-
rosion inhibitors for iron in HCl: cetyltrimethyl ammonium
bromide and tetraphenyl phosphonium chloride,” Corrosion
Prevention and Control, vol. 42, no. 2, pp. 30–34, 1995.
 B. V. Savithri and S. M. Mayanna, “Tetrabutyl ammonium
iodide, cetyl pyridinium bromide and cetyl trimethyl ammo-
nium bromide as corrosion inhibitors for mild steel in
sulphuric acid,” Indian Journal of Chemical Technology, vol. 3,
no. 5, pp. 256–258, 1996.
 T. Vasudevan, S. Muralidharan, S. Alwarappan, and S. V.
K. Iyer, “The inﬂuence of N-hexadecyl benzyl dimethyl
ammonium chloride on the corrosion of mild steel in acids,”
Corrosion Science, vol. 37, no. 8, pp. 1235–1244, 1995.
 S. Muralidharan, K. L. N. Phani, S. Pitchumani, S. Ravichan-
dran, and S. V. K. Iyer, “Polyamino-benzoquinone polymers: a
new class of corrosion inhibitors for mild steel,” Journal of the
Electrochemical Society, vol. 142, no. 5, pp. 1478–1483, 1995.
 O. Benali, L. Larabi, M. Traisnel, L. Gengembre, and Y. Harek,
“Electrochemical, theoretical and XPS studies of 2-mercapto-
1-methylimidazole adsorption on carbon steel in 1 M HClO4,”
Applied Surface Science, vol. 253, no. 14, pp. 6130–6139, 2007.
 E. S. H. E. Ashry, A. E. Nemr, S. A. Essawy, and S. Ragab,
“Corrosion inhibitors part V: QSAR of benzimidazole and 2-
substituted derivatives as corrosion inhibitors by using the
quantum chemical parameters,” Progress in Organic Coatings,
vol. 61, no. 1, pp. 11–20, 2008.
 K. F. Khaled, “The inhibition of benzimidazole derivatives on
corrosion of iron in 1 M HCl solutions,” Electrochimica Acta,
vol. 48, no. 17, pp. 2493–2503, 2003.
 A. Popova, “Temperature eﬀect on mild steel corrosion in acid
media in presence of azoles,” Corrosion Science, vol. 49, no. 5,
pp. 2144–2158, 2007.
 A. Popova, M. Christov, S. Raicheva, and E. Sokolova,
“Adsorption and inhibitive properties of benzimidazole
derivatives in acid mild steel corrosion,” Corrosion Science, vol.
46, no. 6, pp. 1333–1350, 2004.
 A. Popova, M. Christov, and A. Zwetanova, “Eﬀect of the
molecular structure on the inhibitor properties of azoles on
mild steel corrosion in 1 M hydrochloric acid,” Corrosion
Science, vol. 49, no. 5, pp. 2131–2143, 2007.
 V. S. Sastri, J. R. Perumareddi, M. Lashgari, and M. Elbouj-
daini, “Application of ligand ﬁeld theory in corrosion inhibi-
tion,” Corrosion, vol. 64, no. 4, pp. 283–288, 2008.
 K. Tebbji, A. Aouniti, A. Attayibat et al., “Inhibition eﬃ-
ciency of two bipyrazole derivatives on steel corrosion in
International Journal of Corrosion 7
hydrochloric acid media,” Indian Journal of Chemical Technol-
ogy, vol. 18, pp. 244–253, 2011.
 J. D. Talati, M. N. Desai, and N. K. Shah, “Meta-substituted
aniline-N-salicylidenes as corrosion inhibitors of zinc in
sulphuric acid,” Materials Chemistry and Physics, vol. 93, no.
1, pp. 54–64, 2005.
 T. T¨uken, B. Yazici, and M. Erbil, “The eﬀect of nicotinamide
on iron corrosion in chloride solutions,” Turkish Journal of
Chemistry, vol. 26, no. 5, pp. 735–742, 2002.
 A. A. A. Fattah, E. M. Mabrouk, R. M. A. Elgalil, and M. M.
Ghoneim, “N-heterocyclic compounds as corrosion inhibitors
for Zn in HCl acid solutions,” Bulletin de la Societ´e Chimique
de France, vol. 1, pp. 48–53, 1991.
 S. L. Granese, B. M. Rosales, C. Oviedo, and J. O. Zerbino,
“The inhibition action of heterocyclic nitrogen organic com-
pounds on Fe and steel in HCl media,” Corrosion Science, vol.
33, no. 9, pp. 1439–1453, 1992.
 H. A. Al-Lohedan, E. Khamis, and Z. A. Issa, “Studies on the
inﬂuence of temperature on the adsorption of some cationic
surfactants on to steel,” Adsorption Science and Technology, vol.
13, no. 3, pp. 137–152, 1996.
 L. G. Qiu, A. J. Xie, and Y. H. Shen, “A novel triazole-based
cationic gemini surfactant: synthesis and eﬀect on corrosion
inhibition of carbon steel in hydrochloric acid,” Materials
Chemistry and Physics, vol. 91, no. 2-3, pp. 269–273, 2005.
 B. G. Ateya, B. E. El-Anadouli, and F. M. El-Nizamy, “The
eﬀect of thiourea on the corrosion kinetics of mild steel in
H2SO4,” Corrosion Science, vol. 24, no. 6, pp. 497–507, 1984.
 A. S. Fouda, M. N. Mousa, F. I. Taha, and A. I. Elneamaa, “The
role of some thiosemicarbazide derivatives in the corrosion
inhibition of aluminum in HCl,” Corrosion Science, vol. 26, no.
9, pp. 719–726, 1986.
 A. Nahl´e, “Eﬀect of temperature on the corrosion inhibition
of carbon steel in HCl solutions,” Bulletin of Electrochemistry,
vol. 17, no. 5, pp. 221–226, 2001.
 A. Nahl´e, “Inhibition of corrosion of iron in HCl solution
by semicarbazides and thiosemicarbazides,” Bulletin of Electro-
chemistry, vol. 21, no. 6, pp. 275–281, 2005.
 S. N. Raicheva, B. V. Aleksiev, and E. I. Sokolova, “The eﬀect
of the chemical structure of some nitrogen- and sulphur-
containing organic compounds on their corrosion inhibiting
action,” Corrosion Science, vol. 34, no. 2, pp. 343–350, 1993.
 S. H. Sanad, A. A. Ismail, and A. A. El-Meligi, “The eﬀect
of temperature on the corrosion and corrosion inhibition
of steel alloys in hydrochloric acid solutions,” Bulletin of
Electrochemistry, vol. 11, no. 10, pp. 462–469, 1995.
 F. Zucchi, G. Trabanelli, and G. Brunoro, “The inﬂuence of the
chromium content on the inhibitive eﬃciency of some organic
compounds,” Corrosion Science, vol. 33, no. 7, pp. 1135–1139,
 Y. L. Huang, C. N. Cao, M. Lu, and H. C. Lin, “Inhibition
eﬀects of I−
and I2 on stress corrosion cracking of stainless
steel in acidic chloride solutions,” Corrosion, vol. 49, no. 8, pp.
 A. Popova, M. Christov, and T. Deligeorgiev, “Inﬂuence
of the molecular structure on the inhibitor properties of
benzimidazole derivatives on mild steel corrosion in 1 M
hydrochloric acid,” Corrosion, vol. 59, no. 9, pp. 756–764,
 M. Scendo and M. Hepel, “Inhibiting properties of benzimida-
zole ﬁlms for Cu(II)/Cu(I) reduction in chloride media stud-
ied by RDE and EQCN techniques,” Journal of Electroanalytical
Chemistry, vol. 613, no. 1, pp. 35–50, 2008.
 M. Yamaguchi, H. Nishihara, K. Aramaki, M. Tomihari, and
S. Furuya, “The inhibitive eﬀect of organic cations on passive
ﬁlm breakdown of iron in a chloride-containing borate buﬀer
solution,” Corrosion Science, vol. 36, no. 7, pp. 1133–1141,
 A. S. Fouda, A. Abd El-Aal, and A. B. Kandil, “The eﬀect of
some phthalimide derivatives on the corrosion behaviour of
copper in nitric acid,” Anti-Corrosion Methods and Materials,
vol. 52, no. 2, pp. 96–101, 2005.
 K. Kobayashi, K. Shimizu, and M. Iida, “Structural eﬀects of
organic compounds as corrosion inhibitors for hydrogen entry
into iron in sulphuric acid,” Corrosion Science, vol. 35, no. 5-8,
pp. 1431–1435, 1993.
 L. D. Skryler, E. A. Streltsova, and T. L. Skryleva, “Hydrocar-
bon chain length and their eﬀect on corrosion inhibition by
alkylammonium chlorides,” Protection of Metals USSR, vol. 27,
no. 6, pp. 755–758, 1991.
 A. Nahl´e, I. Abu-Abdoun, and I. Abdel-Rahman, “Electro-
chemical studies of the eﬀect of trans-4-hydroxy-4 -stilbazole
on the corrosion inhibition of mild steel in HCl solution,”
Anti-Corrosion Methods and Materials, vol. 54, no. 4, pp. 244–
 A. Nahl´e, I. Abu-Abdoun, and I. Abdel-Rahman, “Inhibition
of carbon steel corrosion by 4-vinylbenzyl triphenyl phospho-
nium chloride in HCl solution,” Anti-Corrosion Methods and
Materials, vol. 55, no. 4, pp. 217–224, 2008.
 A. Nahl´e, I. Abdel-Rahman, and M. Alfarouk, “Eﬀect of
temperature on the inhibition of corrosion of carbon steels
by semicarbazides and thiosemicarbazides,” Bulletin of Electro-
chemistry, vol. 21, no. 8, pp. 353–361, 2005.
 U. Kumar, T. Kato, and J. M. J. Fr´echet, “Use of intermolecular
hydrogen bonding for the induction of liquid crystallinity
in the side chain of polysiloxanes,” Journal of the American
Chemical Society, vol. 114, no. 17, pp. 6630–6639, 1992.
 B. D. Shaw and E. A. Wagstaﬀ, “26. The reaction between
2-picoline and aromatic aldehydes,” Journal of the Chemical
Society (Resumed), pp. 77–79, 1933.
 W. C. Frank, Y. C. Kim, and R. F. Heck, “Palladium-catalyzed
vinylic substitution reactions with heterocyclic bromides,”
Journal of Organic Chemistry, vol. 43, no. 15, pp. 2947–2949,
 D. W. Bruce, S. C. Davis, D. A. Dunmur, S. A. Hudson, P.
M. Maitlis, and P. Styring, “Mesomorphic metal complexes
derived from 4-alkyloxystilbazoles,” Molecular Crystals and
Liquid Crystals Science and Technology Section A, vol. 215, no.
2, pp. 1–11, 1992.